Creep results of NiO, CoO and FeO*.
This chapter presents a comprehensive review of the creep technique used for the study of defect structure and diffusion in metal oxides, both single crystals and ceramics. At high temperatures, the creep rate is proportional to the diffusion coefficient of the slowest species in solid compounds, whatever deformation mechanisms are present (Nabarro viscous creep, recovery creep or pure climb creep). The creep rate dependence on deviation from stoichiometry can be determined from this diffusion. In the case of metal oxides, the departure from stoichiometry is controlled by the oxygen activity which usually is identified with oxygen partial pressure, pO2. The pO2 dependence of the creep rate provides direct information about the nature of minority point defects. On the other hand, studies of the temperature dependency of the creep rate inform us about the activation energy of the diffusion coefficient.This review focuses primarily on the creep behavior of transition metal oxides such as Ni1−yO, Co1−yO, Fe1−yO exhibiting disorder in metal sublattice, as well as ZrO2−x with majority defects in oxygen sublattice. The advantage of these studies is determination of both defect structure and diffusion coefficients of minority defects namely in oxygen sublattice in iron-triad oxides and in zirconium ZrO2 sublattice.
- high temperature creep of metal oxides
- defect structure
This chapter presents a review of the creep technique used for the study of defect structure and diffusion in metal oxides. Transition metals of the iron-row triad (Fe, Co, Ni) monoxides were chosen. These oxides at higher temperatures exhibit electronic conductivity. Zirconia stabilized with yttria, termed as YSZ, was also the subject of interest. This material is treated as model system of ionic (super ionic) conductor. Taking into account that creep behavior of the oxides is generally dependent of the minority defects properties (types and concentrations) which are especially strictly related with majority point defect, a short description of the point defect structure of each analyzed oxide proceeds the appropriate chapter.
2. Definition of terms
Creep, or more generally high-temperature plastic deformation of metal oxides, is a suitable method for measuring diffusion coefficients and to assess the nature of point defects responsible for diffusion processes. Above a so called Tamman’s temperature and under constant applied stress, a steady state is reached where the rate of deformation remains constant. Tamman’s temperature of metal oxides assumes value of about 0.45 × Tmelt [K]  creep rates, , is commonly expressed by the equation 
where ε is the creep strain, A is constant dependent of the material structure and the creep mechanism, σ is the applied stress, m and b are exponents dependent on the creep mechanism, d is the grain diameter, k is Boltzmann’s constant, T is the absolute temperature and Q is an activation energy of the creep.
At high temperatures, the creep rate is proportional to some diffusion coefficient, whatever the exact nature of deformation mechanism: Nabarro-Hearing creep, grain boundary sliding and dislocation movements are valid . This diffusion coefficient, D, is an effective diffusivity involving both the lattice and the grain boundaries diffusivities. In most cases, it reduces to the diffusivity of the slowest species. In case of transition metal oxides, the creep rate dependence on deviation from stoichiometry is carried out through diffusivity. In binary oxides, at high temperatures the deviation from stoichiometry and related majority point defects are controlled by the oxygen partial pressure, pO2. In most cases, these defects are only located either in metal or oxygen sublattice. Defects on other sublattice are present in a much lower concentration (named as ‘minority defects’), and the diffusivity of the corresponding species is very low. Their diffusion coefficient is proportional to the concentration of minority defects, which also varies as some characteristic power law with pO2, so that creep rate has related to this variable. Accordingly, the pO2 dependence of the creep rate leads to a direct approach to assess the nature of the minority point defects 
where , Eact = Q is the energy activation of diffusion and n is the parameter dependent of the point defect structure.
3. Creep of transition metal monoxides
The transition metal monoxides such as iron-triad group (Fe, Co, Ni) show only metal deficiency: Fe1−yO, Co1−yO and Ni1−yO. The nonstoichiometry and related point defect structure discussed below for these oxides are based on both thermogravimetric equilibration and electrochemical measurements. The nonstoichiometry, y, is most pronounced with Fe1−yO (y = 0.043−0.167) [4, 5], whereas in Co1−yO  and Ni1−yO  y is about 0.000–0.012 and 0.0000–0.0010, respectively.
Nonstoichiometry y in M1−yO (M = Fe, Co, Ni) can be modified by changes of oxygen activity, pO2, in thermodynamic equilibrium with the oxide crystal (Kröger and Vink  notation of defects is used throughout this paper):
where i = 0, 1, 2 denotes the degree ionization. The nonstoichiometry of the M1−yO is then given by:
Applying the mass action law to reaction (3) and assuming that interaction among defects may be neglected, as well as supposing appropriate electroneutrality conditions, one arrives at the following relationship between nonstoichiometry and equilibrium oxygen pressure and temperature:
where 1/ny, or simply ny, is the parameter depending on the ionization degree of cation vacancies, assuming 2, 4 and 6 values for neutral, single- and double-ionized vacancies, respectively; Ey denotes the temperature coefficient directly related to the enthalpy of defect formation.
M1−yO (M = Fe, Co, Ni) are p-type semiconductors, which electrical conductivity is realized by electron (or electron hole) hopping mechanism between M3+ and M2+ ions. The concentration of quasi-free electron holes [h•] is given by:
Accordingly, the following relationship between electrical conductivity, σ and equilibrium oxygen pressure and temperature is given by:
where e is the elementary charge, μ is mobility of the holes, σo and ho are constants involving mobility of electron holes and entropy terms of the equilibrium constant of the reaction (3), nσ is the parameter depending on the ionization degree of cation vacancies, assuming ∝, 4 and 6 values for neutral, single- and double-ionized vacancies, respectively; Eσ denotes the activation energy of the electrical conductivity.
Several minority defects can be proposed in M1−yO. Considering only simple defects oxygen vacancies (j = 1 or 2) or oxygen interstitials (k = 1 or 2) the formation of these defects is described by the following:
Applying the mass action law to these equilibriums and taking into account the Eq. (7b), we can write the following relationships:
So, using Eqs. (12) and (13) or Eqs. (14) and (15) carrying out the creep rates measurements as a function of oxygen partial pressure and temperature, we can determine both parameters n and Eact. Then, using the values of electrical properties such as electrical conductivity (or Seebeck coefficient) which are related to the concentration of the electron holes, we can identify the type of minority defect responsible for the creep diffusion process and can determine the activation energy of the diffusion.
3.1. Creep of NiO
Nickel oxide is a nonstoichiometric compound with a deficit of metal. Its chemical formula may be written as Ni1−y.O. The resulting majority point defects are nickel vacancies formula may be written as Ni1−y.O. The resulting majority point defects are nickel vacancies: VNi′, VNi″ and electron holes (Figure 1) . The dependence of electrical conductivity, σ, as a function of oxygen partial pressure, pO2 and temperature is shown in Figure 2 [9, 10]. The reciprocal of oxygen exponent nσ = nh varies values between 4 and 6.
The results of the creep studies of NiO single crystals [11, 12] and NiO polycrystals [3, 13, 14] are summarized in Table 1. The comparison of the activation energies for creep rate with oxygen self-diffusion obtained by Dubois et al. [15, 16] agrees only with a rather large uncertainty [17–19]. Controversy, Figure 3 presents the diffusion coefficients determined by tracer of nickel [17, 18] and by the tracer self-diffusion of oxygen  on one hand, and the diffusion coefficient determined using the creep technique, on the other. The excellent agreement is observed between oxygen diffusion coefficient and the diffusion coefficient from the creep.
|Material||T/Tm**||σ (MPa)||pO2 (Pa)||m||Eact (eV)||n||Minority defect||Mechanism of creep||Ref.|
|NiO s.crystal||0.09–0.66||20–100||0.1–2 × 104||NA||NA||NA||NA||NA|||
|NiO s.crystal||0.6–0.8||15–120||1–2 × 104||12|
|5.4–8.5||−0.06 to +0.11||VO••||Thermally activated glide recovery creep|||
|1–2 × 104||1.5|
|NiO polycrytals||0.56–0.61||34.5–79.8||2 × 104||3.25 ± 0.18||2.46 ± 0.31||NA||NA||Diffusion controlled climb glide|||
|CoO s.crystal||0.49–0.66||6.9–31||2.1 × 104|
1.1 × 10−4
|CoO s.crystal||0.61–0.75||8.3–14.5||NA||5||2.2||NA||NA||Diffusion controlled dislocation motion|||
1 × 105
2 × 104
|CoiO polycrytals||0.58–0.62||34.5–79.8||2 × 104||3||3.12||NA||Na||Dislocation motion|||
|FeO polycrystals||0.73–0.95||2.5–15||10−10–3 × 10−8||4.15 ± 0.10||2.8||NA||VO••||Climbing dislocations|||
|3.2–5.3||3 × 10−13–2 × 10−6||5.3|
|3.0 ± 0.4||−0.015|
3.2. Creep of CoO
Taking into account both crystal structure and nonstoichiometry departure, CoO shows similarities to NiO. However, there is a major difference at low temperature (below 1170 K) and high oxygen pressure CoO is unstable and transforms to the spinel-type Co3O4 (Figure 4). Also the departure of stoichiometry, y, in Co1−yO is about 10 times higher than that of Ni1−yO. Traditional analysis of point defect structure in Co1−yO based on the ideal defect model with the assumption that point defects in Co1−yO are randomly distributed and do not interact with each other, leads to the conclusion that at high pO2 (close to CoO/Co3O4 border) the predominant ionic point defects are VCox and VCo′; at the intermediate region of pO2 both VCo′ and VCo″ coexist together as the predominant ionic point defects; and finally near the border Co/CoO the doubly ionized cobalt vacancies VCo″ are predominant . However, the assumption of validity of ideal point defects in CoO is questionable. The ideal point defect model gives satisfactory results when nonstoichiometry departure and related point defect concentration is below 0.1 at%, for higher concentrations interaction between defects must be taken into account .
The interaction between defects in Co1−yO can be well described by the Debye-Hückel approach . In addition, the model proposed is based on the assumption that the only type of predominant ionic defects present in cobalt monoxide at elevated temperatures are double-ionized cation vacancies, VCo″ instead of two or even more types of ionic defects considered before. Despite the simplicity of the model, the agreement with the experiment is very good within the entire range of CoO stability.
Apart from the Debye-Hückel model, there is also another model making allowance for interaction between the defects which explains well the experimental data of CoO, in particular at high values of deviation from stoichiometric composition (i.e. close to the Co1−yO/Co3O4. This so called cluster model involves the formation of 4:1 clusters consisting of four double-ionized octahedral cobalt vacancies and one trivalent Co ion in tetrahedral interstitial position: [(
The results of the creep studies of CoO single crystals [24–28] and CoO polycrystals  are summarized in Table 1. A comparison of the activation energies for creep rate with oxygen self-diffusion obtained by Dubois et al. [15, 16] agrees only with a rather large uncertainty.
3.3. Creep of FeO
Iron monoxide, termed also as wüstite, has the NaCl-type structure. Compared to other binary oxides of iron-row metals, the wüstite phase exhibits the highest deviation from stoichiometry, varying from 4.3 at% at the Fe/Fe1−yO phase boundary up to 16.7 at% at the Fe1−yO/Fe3O4 interphase (Figure 6) [4, 5, 29]. The non-stoichiometry occurs because of the ease of oxidation of Fe2+ to Fe3+effectively replacing a small portion of Fe2+ with two-thirds their number of Fe3+, which take up tetrahedral positions in the close packed oxide lattice. The considerable concentration of defects, resulting from nonstoichiometry, leads to their strong interactions and formation of complexes. On the basis of neutron diffraction studies, Roth  has proposed the formation of defect complexes composed of two iron vacancies and interstitial iron . This defect is similar to an element of the spinel structure of magnetite Fe3O4. Therefore, the Roth complexes can be formally considered as a magnetite-type defect or a submicrodomain of Fe3O4 in FeO [28, 31]. On the basis of X-ray studies, Koch and Cohen  have postulated that defects in Fe1−yO form associates even larger than Roth 2:1 complexes, composed of 13 iron vacancies and 4 interstitials (termed as cluster 13:4). The formation of the clusters was later confirmed by the neutron diffraction studies of Cheetham et al. [33, 34]. Catlow et al. [35, 36] using the computer simulation method have proposed various kinds of defect clusters such as 4:1, 6:2. 8:3, 10:4, 12:4 and 16:5. It has been postulated that the 4:1 cluster is a constructional unit in formation of higher order clusters. The cluster 16:5 resembles the magnetite structure and can be considered as a Fe3O4-type microdefect.
The creep studies of FeO single crystals were performed by Ilschner et al.  and by Jolles and Monty . The required parameter (where α is Seebeck coefficient) needed to interpretation of the creep rate versus pO2 is presented in Figure 7. The results of the creep studies are summarized in Table 1.
4. Zirconia-based materials
Zirconium dioxide, ZrO2 has three polymorphic modifications: monoclinic below 1440 K, tetragonal 1440–2640 K and cubic above 2640 K. The transition between them involves a large volume expansion cause a cracking upon cooling from high temperature, which is detrimental to the materials structural applications. The destructive phase transformation can be suppressed by total or partial stabilization of high temperature modifications (cubic or tetragonal form). This stabilization consists on the addition to ZrO2 several mole % of MgO, CaO or Y2O3 among others. The most popular stabilizer is Y2O3 termed as yttria.
Yttria-stabilized zirconia (YSZ) ceramics is a strategic functional material which has found extensive applications in electrochemical devices, such as gas sensors, solid oxide fuel cells and electrolysis cells.
Also the YSZ well known as an excellent construction material due to such properties as: high hardness, low wear resistance, low coefficient of friction, high elastic modules, chemical inertness, low thermal conductivity and high melting point [39–42]. It is also recognized that the useful mechanical properties are obtained in multiphase material known as partially stabilized zirconia (PSZ). Garvie and Nicholson  have demonstrated that a fine-scale precipitate of monoclinic zirconia in a cubic stabilized matrix enhances the strength of PSZ. Very interested mechanical properties were discovered in fine-grained tetragonal ZrO2 stabilized with 3 mol% Y2O3 termed as 3Y-TZP [44, 45]. The macroscopic and microscopic behavior of 3Y-TZP can be characterized as structural or micrograin superplasticity, according to the definition used by metallurgists. The 170% elongation reported by Wakai et al.  on 3Y-TZP has been considered as evidence of ceramic superplasticity in the ceramic materials. 3Y-TZP, termed as ‘ceramic steel’ [46, 47], is now considered to be the model ceramic system. The fine grade size leads to a very dense, non-porous ceramic with excellent mechanical strength, corrosion resistance, impact toughness, thermal shock resistance and very low thermal conductivity. Due to its characteristics Y-TZP is used in wear parts, cutting tools and thermal barrier coatings.
Also, electrical properties of 3Y-TZP are very interesting. At moderate temperatures below 970 K the grain interior of Y-TZP has higher conductivity [47, 48] than that of fully (YSZ) or partially stabilized (PSZ) zirconia . However, the total conductivity of Y-TZP is lower due to the high contribution of grain boundary resistivity, known as the blocking effect [47, 49]. It was found that addition of Al2O3 leads considerable reduction of the blocking effect .
4.1. Defect structure of YSZ
The defect reactions in the yttria-stabilized zirconia can be written as:
The majority defect oxygen in yttria-stabilized zirconia are oxygen vacancies and yttrium ions Y3+ (using defect notation) occupying zirconium positions the electroneutrality conditions is given by:
The possible minority defects are: zirconium interstitials and zirconium vacancies . They occupy positions in zirconium sublattice and form according to the following reactions:
4.2. Creep of single crystalline zirconia
Marcartney et al.  studied creep of single crystal zirconia stabilized with 12 mol% CaO within 1623–1723 K. They observed considerable climb and glide formation. Dominguez-Rodriguez et al. [53–56] examined cubic YSZ (9.4–18 mol% Y2O3) single crystals. The determined activation energies of the deformation process were 646.4; 800.8 and 944.7 kJ/mol for 9.4, 12 and 18 mol% of yttria, respectively. Lankford  studied the deformation of two single crystals of YSZ containing 2.8 and 12 mol% Y2O3.The temperature range of the experiments was 296–1423 K. The plastic flow with rapid decrease in strength with increasing temperature was observed. The deformation was attributed to dislocation activity alone. Corman  examined the creep of single crystal 9.5 mol% yttria partially stabilized zirconia, within temperature range 1923–2123 K and stress from 12.5 to 100 MPa.
The stress exponent, m, and activation energy Q (Eq. (1)) were m = 4 and Q = 436 kJ/mol. This value is close to the lattice diffusion of Zr (418 kJ/mol). So, he concluded that cation diffusion is controlled the process deformation.
4.3. Creep of polycrystalline zirconia
The dependence of steady state creep rate, ; on stress, σ; temperature, T and grain size, d of polycrystalline zirconia is given by a general relationship of the form:
where A is a dimensionless constant, G is the shear modulus, b is the Burgers vector, k is Boltzmann’s constant, p and m are constants termed the inverse grain size and stress exponent, respectively and D is the appropriate diffusion coefficient given by:
where Do is a frequency factor, Q is the appropriate activation energy and R is the gas constant.
Creep of polycrystalline zirconia was recently intensively studied. The subjects of interest were cubic stabilized zirconia, CSZ [59–64], partial stabilized zirconia, PSZ [65–67] as well as tetragonal zirconia polycrystals, TZP [44, 68–73].
St Jacques and Angers  examined zirconia stabilized with 18 mol% CaO in the temperatre range 1470–1670 K and stress between 3.5 and 27.5 MPa. The parameter m in Eq. (26) was equal to 1, which suggested diffusionally controlled creep. The detailed study by Dimos and Kohlstedt  on a cubic 25YSZ indicated that the creep is controlled by the Nabarro-Herring diffusion mechanism with parameters m ≈ 1 and p ≈ 2. Wakai et al. [61, 63] reported that a stress exponent m ≈ 2 in an 8YSZ. Sharif et al.  studying a static grain growth claimed that cubic zirconia is prone to extensive grain growth.
Evans  studied deformation of yttria- and scandia- partially stabilized zirconia, PSZ (1436 < T < 1808 K; 4.1 < σ < 7.1 MPa). The activation energies were 373 and 360 kJ/mol for scandia and yttria, respectively, the parameter p = 2 was found, the parameter m was 1.5 for scandia stabilized zirconia and it assumed two values m = 1 and m = 6 for yttria. Seltzer, and Talty  studied Y-PSZ at high temperatures (up to 2270 K), they found m = 1.5 for fine-grained samples (d varied from 15 to 20 μm) and activation energy was 531 kJ/mol. Chevalier et al.  studied PSZ materials stabilized by MgO, they concluded that cavitations and microcracking by grain boundary sliding have been identified as the main creep mechanisms.
Wakai et al.  examined creep of 3Y-TZP within temperature range of 1423–1723 K. The stress exponents m = 1.5 at 1423 K and gradually increased with temperature reaching value m = 1.9 at 1723 K. The activation energy was 586 kJ/mol. Nauer and Carry  investigated the creep behavior TZP containing 2, 3 and 4 mol% Y2O3. At lower stresses (σ < 10 MPa) the parameters were: m = 2.4 and p = 1 and activation energy Q = 590 kJ/mol. At higher stresses ca. 100 MPa, the parameter m = 1. Authors proposed two different deformation regimes: an interface reaction controlled creep at low stresses and a grain boundary diffusion controlled creep at high stresses. Lakki et al.  studied 2Y-TZP material using two techniques the creep and the internal friction (it consists on applying a cyclic stress σ = σo cos (ωt) to a sample and measuring its response in the form of strain, ε). Both techniques provide at low stresses (< 15 MPa) close values of the activation energies and lead to conclusion that grain boundary sliding is the main deformation mechanism. Owen and Chokshi  and Chokshi  investigated 3Y-TZP. The experimental data over a wide range of stresses revealed a transition in stress exponent. Deformation at low and high stress regions was associated with m ≈ 3, p ≈ 1 and m ≈ 2, p ≈ 3, respectively. The activation energy was Q = 550 kJ/mol for both regions. Authors postulated that the interface reaction is controlled at low stress region and the grain boundary sliding at high stress region. Ghosh et al.  examined effect of silica additions on creep behavior of 3Y-TZP. The determined results were verified by tracer diffusion measurements. The creep data at high stresses are consisted with Coble diffusion and creep at lower stresses is attributed to interface-controlled diffusion mechanism. Addition of silica has only minor effect on both grain boundary and lattice diffusion. Ghost and Chokshi  studied the creep of nanocrystalline 3Y-TZP who obtained results indicating the same deformation mechanism as for micro-sized materials. Liu et al.  examined creep behavior of zirconia stabilized with 2.5 mol%. They postulated the grain boundary sliding accompanied by intergranular dislocation due to existence of amorphous phases.
The emphasis of this review was to compile existing data in the creep behavior of two types of oxides: iron-row group M1−yO (M = Ni, Co, Fe) which properties are strongly related with the oxygen partial pressure (pO2) dependent departure from stoichiometry (y) and superionic ZrO2-based materials. Two different approaches to creep methodology are used. In case of the transition metal oxides such as M1−yO the creep experiments required determination of the rate deformation () as a function σ, T, pO2 and grain size (d) for polycrystalline materials. On the other hand, the oxide superionics such as stabilized zirconia concentration of ionic defects () is fixed by the amount used stabilizer (usually Y2O3). Electronic defects (e′ and h•) play role only in the extremely reduced or oxidizing conditions (usually very hard to achieve experimentally). Therefore, the creep rate is studied as a function σ, T and d in case of the polycrystals.
From this review several general trends in creep behavior emerge. Deformation of single crystals is typically controlled by dislocation glide on the most favorable slip system. On the other hand, deformation of polycrystalline oxides is controlled by diffusion of the slowest species along the fastest path, such as through the lattice, along grain boundaries or through a second phase formed at the grain boundaries. Dislocations play a more or less important role depending on the specific oxide.
Steady state creep of M1−yO appears to be controlled by oxygen diffusion through either oxygen vacancies or interstitials. On the other hand in case of stabilized zirconia it is controlled by cation diffusion (Zr4+ or Y3+). In any cases diffusion, involving both lattice and grain boundary data are needed to verification of proposed mechanisms. Recently used secondary ion mass spectrometry (SIMS) is suitable for this purpose [73, 76–78].
This work was financially supported by the National Science Centre of the Republic of Poland, under Grant No 2016/23/B/ST8/00163. One of the author (MR) would like to thank to Professor J. Philibert- Head of the Laboratoire de Physique des Materiaux CNRS Bellevue and his coworkers: Dr. J. Castaing, Dr. C. Monty and Dr. E. Jolles for the opportunity to perform studies on creep of single crystals FeO in their labs.
Ashby M. Materials. Oxford: Elsevier; 2014. p. 336
Bretheau T, Castaing J, Rabier J, Veyssiere P. Dislocations motion and high temperature plasticity of binary and ternary oxides. Advances in Physics. 1979; 28:835
Philibert J. Creep and diffusion. Solid State Ionics. 1984; 12:321-336
Rekas M, Mrowec S. On defect clustering in the wustite phase. Solid State Ionics. 1987; 22:185-197
Nowotny J, Rekas M. Defect structure and thermodynamic properties of the wustite phase (Fe1-yO). Journal of the American Ceramic Society. 1989; 72:1221-1228
Dickmann R. Cobaltous oxide point defect structure and non-stoichiometry, electrical conductivity, cobalt tracer diffusion. The Journal of Physical Chemistry. (Munich. 1977; 107:189-210
Nowotny J, Rekas M. Seebeck effect of undoped and Cr-doped NiO. Solid State Ionics. 1984; 12:253-261
Kröger FA, Vink HJ. In: Seitz F, Turnbull D, editors. Solid State Physics. Vol. 3. New York: Academic Press; 1956. p. 307
Bransky I, Tallan NM. High temperature defect structure and electrical properties of NiO. The Journal of Chemical Physics. 1968; 49:1243-1249
Farhi R, Petot-Ervas G. Thermodynamic study of point defects in single crystalline nickel oxide. Analysis of experimental results. Journal of Physics and Chemistry of Solids. 1978; 39:1175-1179
Domingues-Rodrigueez A, Castaing J, Philibert J. Plastic deformation of pure and doped Nio single crystals. Materials Science and Engineering. 1977; 27:217-223
Carrera-Caño J, Domingues-Rodrigueez A, Marquez R, Castaing J, Philibert J. Point defects and high-temperature creep of non-stoichiometric NaCl-type oxide single crystals. I, NiO. Philosophical Magazine A. 1982; 46:397-407
Jimenez-Melendo M, Cabrera-Cano J, Dominguez-Rodriguez A, Castaing J. Pure diffusional creep of NiO polycrystals. The Journal of Physical Chemistry Letters. 1983; 44:L-339-L-343
Krishinamachri V, Notis MR. High temperature deformation of polycrystalline NiO and CoO. Acta Metallurgica (pre 1990). 1977; 25:1307
Dubois C, Monty C, Philibert J. Oxygen self- diffusion in NiO single crystals. Philosophical Magazine A. 1982; 46:419-433
Dubois C, Monty C, Philibert J. Influence of oxygen pressure on oxygen self-diffusion in NiO. Solid State Ionics. 1984; 12:75-78
Choi JS, Moore WJ. Diffusion of nickel in single crystals of nickel oxide. The Journal of Physical Chemistry. 1962; 66:1308-1311
Lindner RL, Akerstro A. Diffusion of nickel-63 (NiO). Discussions of the Faraday Society. 1957; 23:133-136
O’Keeffe M, Moore WJ. Diffusion of oxygen in single crystal of nickel oxide. The Journal of Physical Chemistry. 1961; 65:1435-1439
Nowotny J, Rekas M, et al. Journal of the American Ceramic Society. 1989; 72:1199-1207
Stoneham AM, Tomlison SM, Catlow CRA, Harding JH. Clustering of defects. In: Adles D, Fritsche H, Ovshinsky SR, editors. Physics of Disordered Materials. New York: Plenum Press; 1985. p. 243-252
Nowotny J, Rekas M. Defect structure of cobalt monoxide. II. The Debye-Hückel Model. Journal of the American Ceramic Society. 1989; 72:1207-1214
Nowotny J, Rekas M. Defect structure of cobalt monoxide. III. The cluster model. Journal of the American Ceramic Society. 1989; 72:1215-1220
Clauer AH, Selzer MS, Wilcox BA. Creep of CoO single-crystals. Journal of Materials Science. 1971; 4:1379-1388
Krishinamachri V, Jones JT. Compressive creep of CoO single crystals. Journal of the American Ceramic Society. 1974; 57:506-507
Nehring VW, Smyth JR, McGee TD. Compressive creep of CoO single crystals. Journal of the American Ceramic Society. 1974; 60:328-332
Routbort JL. The stoichiometry dependence of the deformation of Co1-δO. Acta Metallurgica. 1982; 30:663-671
Dominguez-Rodriguez A, Sanchez M, Marquez R, Castaing J, Monty C, Philibert J. Point defects and high-temperature creep of non-stoichiometric NaCl-type oxide single crystals. II CoO. Philosophical Magazine A. 1982; 46:411-418
Darken LS, Gurry RW. The system iron-oxygen II Equilibrium and thermo-dynamics of liquid oxide and other phases. Journal of the American Chemical Society. 1946; 68:798-812
Roth WL. Defects in the crystals and magnetic structure of ferrous oxide. Acta Crystallographica. 1960; 13:140-149
Nowotny J, Rekas M, Wierzbicka M. Defect structure and electrical properties of the wustite phase. Zeitschrift für Physikalische Chemie. 1982; 131:191-198
Koch FB, Cohen JB. Defect structure of Fe1-yO. Acta Crystallographica Section B. 1969; 25:275-287
Cheetham AK, Fender BEF, Taylor RI. High temperature neutron diffraction study of Fe1-yO. Proceedings of the Physical Society. London, Solid State Physics. 1971; 4:2160-2165
Battle PD, Cheetham AK. The magnetic structure in non-stoichiometric ferrous oxide. Journal of Physics C. 1979; 12:337-345
Catlow CRA. Defect clustering in non-stoichiometric oxides. In: Sørensen T, editor. Nonstoichiometric Oxides. New York: Academic Press; 1981. p. 61-98
Stoneham AM, Tomlinson SM, Catlow CRA, Hardings JH. Defect clustering in rock-salt structured transition metal oxides. In: Simkovich G, Stubican VS, editors. Transport in Non-Stoichiometric Compounds. New York: Plenum Press; 1985. p. 243-252
Ilschner B, Reppich B, Riecke E. High-temperature steady-state creep and atomic disorder in ironII oxide. Discussions of the Faraday Society. 1964; 38:243-250
Jolles E, Monty C. High temperature creep of Fe1-xO. Philosophical Magazine A. 1991; 64:765-775
Badwal SPS, Bannister MJ, Hannik RHJ, editors. Science and Technology of Zirconia V. Basel: Technocomic Publ. Comp.; 1993
Somiya S, Yamamoto N, Yanagida H, editors. Science and Technology of Zirconia III. Westerville, OH (USA): American Ceramic Society Inc; 1988
Claussen N, Ruhle M, Heuer AH, editors. Science and Technology of Zirconia, II. Columbus, OH (USA): American Ceramic Society, Inc; 1983
Kisi E. Zirconia Engineering Ceramics. Switzerland: Trans.Tech. Publ. Ltd; 1998
Garvie RC, Nicholson PS. Structure and thermo-mechanical properties of partially stabilized zirconia in the CaO-ZrO2 system. Journal of the American Ceramic Society. 1972; 55:152-157
Wakai F, Sakaguchi S, Matsuno Y. Superplasticity of yttia-stabilized tetragonal ZrO2 polyctrystals. Advanced Ceramic Materials. 1986; 1:259-263
Carry C. In: Kobayashi M, Wakai F, editors. Proceedings of the MRS International Meeting on Advanced Materials, Pittsburgh, PA (USA). 1989; 7:199-215
Garvie RC, Hannik RH, Pacoe RT. Ceramic steel. Nature. 1975; 258:703-704
Badwal SPS. Yttria tetragonal zirconia polycrystalline electrolytes for solid state electrochemical cells. Applied Physics A. 1990; 50:449-462
Badwal SPS, Drennan J. Grain boundary resistivity in Y-TZP materials as a function of thermal history. Journal of Materials Science. 1989; 24:88-96
Meyer D, Eisele U, Satet R, Rödel J. Codoping of zirconia with yttria and Scandia. Scripta Materialia. 2008; 58:215-218
Obal K, Brylewski T, Pedzich Z, Rekas M. Modification of yttria-doped tetragonal zirconia polycrystal ceramics. International Journal of Electrochemical Science. 2012; 7:6831-6845
Weppner W. Electrochemical transient investigations of the diffusion and concentration of electrons in yttria sabilized zirconia-solid electrolytes. Zeitschrift für Naturforschung. 1976; 31a:1336-1343
Mecartney ML, Donlon WT, Heuer AH. Plastic deformation in CaO stabilized ZrO2 (CSZ). Journal of Materials Science. 1980; 15:1063-1065
Dominguez-Rodriguez A, Lagerloff KPD, Heuer AH. Plastic deformation and solid-solution hardening of Y2O3-stabilized ZrO2. Journal of the American Ceramic Society. 1986; 69:281-284
Martinez-Fernandez J, Jimenez-Melendo M, Dominguez-Rodriguez AA. High temperature creep of yttria-stabilized zirconia single crystals. Journal of the American Ceramic Society. 1990; 73:2452
Dominguez-Rodriguez A, Jemenez-Melendo M, Casting J. Plasticity of zirconia. In: Bradt RC, Brookes CA, Routbort JL, editors. Deformation of Ceramics. New York: Plenum Press; 1995. p. 31-41
Gomez-Garcia D, Martinez-Fernandez J, Dominguez-Rodriguez A, Casting J. Mechanizm of high-temperature creep of full stabilized zirconia single crystals as a function of the yttria content. Journal of the American Ceramic Society. 1997; 80:1668-1672
Lankford J. Deformation and fracture of Yttria-stabilized zirconia single crystals. Journal of Materials Science. 1986; 21:1981-1989
Corman GS, High-temperature creep of yttria-stabilized zirconia single crystals. G.E. Research and Development, Technical Information Series. 1989. Ceramics Laboratory, Schenectady NY (USA) #89CRD084
St Jacques RG, Angers R. Creep of CaO-Stabilized ZrO2. Journal of the American Ceramic Society. 1972; 55:571-574
Dimos D, Kohlstedt DL. Diffusional creep and kinetic demixing in yttria-stabilized zirconia. Journal of the American Ceramic Society. 1987; 70:531-536
Chen I-W, Xue LA. Development of superplastic structural ceramics. Journal of the American Ceramic Society. 1990; 73:2585-2609
Wakai F, Nagano T. Effecxt of solute ion and grain size on superplasticity of ZrO2 polycrystals. Journal of Materials Science. 1991; 26:241-247
Wakai F. Step model of solution-precopitation creep. Acta Metallurgica et Materialia. 1994; 42:1163-1172
Sharif AA, Imamura PM, Michell TE, Mecartney ML. Control of grain growth using intergranular silicate phase in cubic yttria-stabilized zirconia. Acta Materialia. 1998; 6:3863-3872
Sudhir B, Chokshi AH. Compression creep characteristics of 8 mol% - yttria-stabilized zirconia. Journal of the American Ceramic Society. 2001; 84:2625-2632
Evans PE. Creep in yttria- and scandia-stabilized zirconia. Journal of the American Ceramic Society. 1970; 53:365-369
Seltzer MS, Talty PK. High temperature creep of Y2O3 – stabilized ZrO2. Journal of the American Ceramic Society. 1975; 58:124-130
Chevalier J, Olagon C, Fantzyyi G, Gros H. Creep behavior of alumina, zirconia and zirconia-toughened alumina. Journal of the European Ceramic Society. 1997; 17:859-864
Nauer M, Carry C. Creep parameters of yttria doped zirconia materials and superplasticity deformation mechanisms. Scripta Metallurgica et Materialia. 1990; 24:1459-1463
Lakki A, Schaller R, Nauer M, Carry C. High temperature siperplastic creep and internal friction of yttria doped zirconia polycrystals. Acta Metallurgica et Materialia. 1993; 41:2845-2853
Owen DM, Hokshi AH. The high temperature mechanical characteristics of super plastic 3 mol% yttria stabilized zirconia. Acta Materialia. 1998; 46:667-679
Chokshi AH. The role of diffusion creep in the superplastic deformation of 3 mol% yttria stabilized tetragonal zirconia. Scripta Materialia. 2000; 42:241-248
Ghosh S, Kilo M, Borchardt G, Chokshi AH. Diffusion and creep in silica-doped tetragonal zirconia. Journal of the American Ceramic Society. 2009; 92:3004-3013
Ghosh S, Chokshi AH. Creep in nanocrystalline zirconia. Scripta Materialia. 2014; 86:13-16
Liu E, Wang H, Xiao G, Yuan G, Shu X. Creep-related micromechanical behavior of zirconia-based ceramics investigated by nanoindentation. Ceramics International. 2015. DOI: 10.1016/j.ceramint 2015.06.136
Bak T, Nowotny J, Prince K, Rekas M, Sorrell CC. Grain boundary diffusion of magnesium in zirconia. Journal of the American Ceramic Society. 2002; 85:2244-2250
Swaroop S, Kilo M, Argirusis C, Borchardt G, Chokshi AH. Lattice and grain boundary diffusion of cations in 3Y-TZP. Analyzed using SIMS. Acta Materialia. 2005; 53:4975-4985
Kowalski K, Obal K, Pedzich Z, Schneider K, Rekas M. Lattice and grain boundary diffusion of Al in tetragonal yttria-stabilized zirconia polycrystalline ceramics (3Y-TZP). Analyzed using SIMS. Journal of the American Ceramic Society. 2014; 97:3123-3127